LMucko/crystallography-open-database huggingface dataset:
Synthesis and structural characterization of sodium vanadyl(IV) orthophosphate NaVOPO4
Lii, K. H.; Li, C. H.; Chen, T. M.; Wang, S. L.; Zeitschrift fur Kristallographie 197 (1991) 67–73; doi:10.1524/zkri.1991.197.14.67

data_8104522
_publ_section_title
;
 Synthesis and structural characterization of sodium vanadyl(IV)
 orthophosphate NaVOPO4
;
_journal_name_full               'Zeitschrift fur Kristallographie'
_journal_page_first              67
_journal_page_last               73
_journal_paper_doi               10.1524/zkri.1991.197.14.67
_journal_volume                  197
_journal_year                    1991
_chemical_formula_sum            'Na O5 P V'
_chemical_formula_weight         184.90
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 115.29(1)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.524(1)
_cell_length_b                   8.455(4)
_cell_length_c                   7.119(1)
_cell_volume                     355.05(19)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_exptl_absorpt_coefficient_mu    3.254
_exptl_crystal_density_diffrn    3.459
_exptl_crystal_F_000             356
_refine_ls_goodness_of_fit_ref   1.195
_refine_ls_number_parameters     74
_refine_ls_number_reflns         568
_refine_ls_R_factor_gt           0.027
_refine_ls_wR_factor_gt          0.030
_cod_data_source_file            Zeit-Krist-1991-197-67-73.cif
_cod_data_source_block           NaVOPO4
_cod_depositor_comments
;
The following automatic conversions were performed:

'_journal_paper_doi' value
'https://doi.org/10.1524/zkri.1991.197.14.67' was changed to
'10.1524/zkri.1991.197.14.67'.

Automatic conversion script
Id: cif_fix_values 6433 2018-09-21 13:16:33Z andrius 
;
_cod_original_sg_symbol_H-M      'P 21/c'
_cod_database_code               8104522
A single-crystal neutron-diffraction study of urea-phosphoric acid
Kostansek, Edward C.; Busing, William R.; Acta Crystallographyca B  (1972) 2454–2459; doi:10.1107/S0567740872006272

data_2108009
_publ_section_title
;
 A single-crystal neutron-diffraction study of urea-phosphoric acid
;
_journal_name_full               'Acta Crystallographyca B'
_journal_page_first              2454
_journal_page_last               2459
_journal_paper_doi               10.1107/S0567740872006272
_journal_volume                  B28
_journal_year                    1972
_chemical_formula_sum            'C H7 N2 O5 P'
_chemical_formula_weight         158.06
_space_group_IT_number           61
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      61
_symmetry_space_group_name_Hall  '-P 2ac 2ab'
_symmetry_space_group_name_H-M   'P b c a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   17.6492(6)
_cell_length_b                   7.4820(3)
_cell_length_c                   9.0018(4)
_cell_volume                     1188.70(8)
_diffrn_ambient_temperature      298
_diffrn_radiation_probe          neutron
_diffrn_radiation_wavelength     1.077
_exptl_absorpt_coefficient_mu    0.223
_exptl_crystal_density_diffrn    1.766
_refine_ls_number_parameters     155
_refine_ls_number_reflns         1926
_refine_ls_R_factor_all          0.114
_refine_ls_R_factor_gt           0.092
_cod_data_source_file            Acta-Cryst-1972-B28-2454-2459.cif
_cod_data_source_block           Urea-Phosphoric-Acid
_cod_depositor_comments
;
The following automatic conversions were performed:

'_journal_paper_doi' value
'https://doi.org/10.1107/S0567740872006272' was changed to
'10.1107/S0567740872006272'.

Automatic conversion script
Id: cif_fix_values 6433 2018-09-21 13:16:33Z andrius 
;
_cod_original_formula_sum        'H7 C N2 O5 P'
_cod_database_code               2108009
Crystal structure determination by powder neutron diffraction at the spallation neutron source, ISIS
Cheetham, A.K.; David, W.I.F.; Eddy, M.M.; Jakeman, R.J.B.; Johnson, M.W.; Torardi, C.C.; Nature 320 (1986) 46–48; doi:

data_1544550
_publ_section_title
;
 Crystal structure determination by powder neutron diffraction at the
 spallation neutron source, ISIS
;
_journal_name_full               Nature
_journal_page_first              46
_journal_page_last               48
_journal_volume                  320
_journal_year                    1986
_chemical_formula_sum            'As Fe O4'
_chemical_name_common            FeAsO4
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 1 21/n 1'
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_cell_angle_alpha                90
_cell_angle_beta                 104.47(1)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.5636(1)
_cell_length_b                   8.0795(1)
_cell_length_c                   5.0117(1)
_cell_volume                     296.550(16)
_cod_data_source_file            FeAsO4.cif
_cod_data_source_block           FeAsO4
_cod_original_formula_sum        'Fe As O4'
_cod_database_code               1544550
Six-fold-coordinated phosphours by oxygen in AlPO4 quartz homeotype under high pressure :Sample at 13.9 GPa
Pellicer-Porres, J.; Saitta, A.M.; Polian, A.; Itie, J.P.; Hanfland, M.; Nature Materials 6 (2007) 698–702; doi:

data_1544551
_publ_section_title
;
 Six-fold-coordinated phosphours by oxygen in AlPO4 quartz homeotype under
 high pressure :Sample at 13.9 GPa
;
_journal_name_full               'Nature Materials'
_journal_page_first              698
_journal_page_last               702
_journal_volume                  6
_journal_year                    2007
_chemical_formula_sum            'Al O4 P'
_chemical_name_common            'AlPO4 CrVO4 structure @ 13.9 GPa'
_space_group_IT_number           63
_space_group_name_H-M_alt        'C m c m'
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.0365(7)
_cell_length_b                   7.2908(9)
_cell_length_c                   5.7491(9)
_cell_volume                     211.11(5)
_cod_data_source_file            AlPO4-Cmcm.cif
_cod_data_source_block           AlPO4_Cmcm
_cod_original_formula_sum        'Al P O4'
_cod_database_code               1544551
Six-fold-coordinated phosphours by oxygen in AlPO4 quartz homeotype under high pressure :Sample at 97.5 GPa
Pellicer-Porres, J.; Saitta, A.M.; Polian, A.; Itie, J.P.; Hanfland, M.; Nature Materials 6 (2007) 698–702; doi:

data_1544552
_publ_section_title
;
 Six-fold-coordinated phosphours by oxygen in AlPO4 quartz homeotype under
 high pressure :Sample at 97.5 GPa
;
_journal_name_full               'Nature Materials'
_journal_page_first              698
_journal_page_last               702
_journal_volume                  6
_journal_year                    2007
_chemical_formula_sum            'Al O4 P'
_chemical_name_common            'AlPO4 monoclinic CaCl2 structure @ 97.5 GPa'
_space_group_IT_number           10
_space_group_name_H-M_alt        'P 1 2/m 1'
_symmetry_space_group_name_Hall  '-P 2y'
_symmetry_space_group_name_H-M   'P 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 87.4(2)
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.838(1)
_cell_length_b                   2.506(5)
_cell_length_c                   4.036(8)
_cell_volume                     38.78(11)
_cod_data_source_file            AlPO4-mCaCl2.cif
_cod_data_source_block           AlPO4_CaCl2
_cod_original_formula_sum        'Al P O4'
_cod_database_code               1544552
Photo-induced magnetization and first-principles calculations of a two-dimensional cyanide-bridged Co-W bimetal assembly.
Miyamoto, Y.; Nasu, T.; Ozaki, N.; Umeta, Y.; Tokoro, H.; Nakabayashi, K.; Ohkoshi, S.; Dalton transactions (Cambridge, England : 2003) 45 (2016) 19249–19256; doi:10.1039/c6dt03793c

data_7041189
_publ_section_title
;
 Photo-induced magnetization and first-principles calculations of a
 two-dimensional cyanide-bridged Co-W bimetal assembly.
;
_journal_issue                   48
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              19249
_journal_page_last               19256
_journal_paper_doi               10.1039/c6dt03793c
_journal_volume                  45
_journal_year                    2016
_chemical_formula_sum            'C18 Br2 Co N10 O2 W'
_chemical_formula_weight         790.840
_chemical_name_common            'Photo-induced phase'
_chemical_name_systematic
;
    ?
;
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_audit_update_record
;
2016-09-23 deposited with the CCDC.
2016-11-14 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 107.35(9)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   13.193(10)
_cell_length_b                   13.949(11)
_cell_length_c                   15.040(12)
_cell_measurement_temperature    13
_cell_volume                     2642(4)
_diffrn_ambient_temperature      13
_diffrn_detector                 'D/tex Ultra'
_diffrn_measurement_device_type  'Ultima IV'
_diffrn_radiation_monochromator  none
_diffrn_source                   'X-ray tube'
_diffrn_source_target            Cu
_exptl_crystal_density_diffrn    1.9883
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             1460.00
_pd_calc_method                  'Rietveld Refinement'
_pd_char_colour                  red
_pd_instr_location               ' ?'
_pd_meas_2theta_range_inc        0.0200
_pd_meas_2theta_range_max        40.0000
_pd_meas_2theta_range_min        5.0000
_pd_meas_number_of_points        1751
_pd_meas_scan_method             step
_pd_proc_2theta_range_inc        0.0200
_pd_proc_2theta_range_max        40.0000
_pd_proc_2theta_range_min        5.0000
_pd_proc_ls_prof_R_factor        0.0033
_pd_proc_ls_prof_wR_expected     0.0037
_pd_proc_ls_prof_wR_factor       0.0044
_refine_ls_goodness_of_fit_all   1.1814
_refine_ls_number_constraints    6
_refine_ls_number_parameters     13
_refine_ls_number_restraints     0
_cod_data_source_file            c6dt03793c2.cif
_cod_data_source_block           Br8_C72_Co4_N40_O8_W4
_cod_depositor_comments
'Adding full bibliography for 7041188--7041189.cif.'
_cod_original_sg_symbol_H-M      'P 21/c'
_cod_database_code               7041189
_rigaku_reference_intensity_ratio 1.56
Crystal structure of potassium borosilicate, K2O*B2O3*4SiO2
Ihara, M.; Kamei, F.; Yogyo-Kyokai-Shi 88 (1980) 32–35; doi:

data_1544559
_publ_section_title
;
 Crystal structure of potassium borosilicate, K2O*B2O3*4SiO2
;
_journal_name_full               Yogyo-Kyokai-Shi
_journal_page_first              32
_journal_page_last               35
_journal_volume                  88
_journal_year                    1980
_chemical_formula_sum            'B K O6 Si2'
_chemical_name_common            KBSi2O6
_space_group_IT_number           220
_space_group_name_H-M_alt        'I -4 3 d'
_symmetry_space_group_name_Hall  'I -4bd 2c 3'
_symmetry_space_group_name_H-M   'I -4 3 d'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   12.60400
_cell_length_b                   12.60400
_cell_length_c                   12.60400
_cell_volume                     2002.282
_cod_data_source_file            KBSi2O6.cif
_cod_data_source_block           KBSi2O6
_cod_original_formula_sum        'K B Si2 O6'
_cod_database_code               1544559
Synthesis and structural study of the KNb4O6-type compound
Sugimoto, W.; Mimuro, K.; Sugahara, Y.; Kuroda, K.; Journal of the Ceramic Society of Japan 107 (1999) 318–321; doi:

data_1544560
_publ_section_title
;
 Synthesis and structural study of the KNb4O6-type compound
;
_journal_name_full               'Journal of the Ceramic Society of Japan'
_journal_page_first              318
_journal_page_last               321
_journal_volume                  107
_journal_year                    1999
_chemical_formula_sum            'K Nb O3'
_chemical_name_common            KNbO3
_space_group_IT_number           35
_space_group_name_H-M_alt        'A 2 m m'
_symmetry_space_group_name_Hall  'A -2 2'
_symmetry_space_group_name_H-M   'A 2 m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   3.9807(7)
_cell_length_b                   5.688(1)
_cell_length_c                   5.711(1)
_cell_volume                     129.31(4)
_cod_data_source_file            KNbO3.cif
_cod_data_source_block           KNbO3
_cod_database_code               1544560
Synthesis and structural study of the KNb4O6-type compound
Sugimoto, W.; Mimuro, K.; Sugahara, Y.; Kuroda, K.; Journal of the Ceramic Society of Japan 107 (1999) 318–321; doi:

data_1544561
_publ_section_title
;
 Synthesis and structural study of the KNb4O6-type compound
;
_journal_name_full               'Journal of the Ceramic Society of Japan'
_journal_page_first              318
_journal_page_last               321
_journal_volume                  107
_journal_year                    1999
_chemical_formula_sum            'K Nb4 O6'
_chemical_name_common            KNb4O6
_space_group_IT_number           123
_space_group_name_H-M_alt        'P 4/m m m'
_symmetry_space_group_name_Hall  '-P 4 2'
_symmetry_space_group_name_H-M   'P 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   4.1396(6)
_cell_length_b                   4.1396(6)
_cell_length_c                   8.256(1)
_cell_volume                     141.48(3)
_cod_data_source_file            KNb4O6.cif
_cod_data_source_block           KNb4O6
_cod_database_code               1544561
Neutron diffraction study on the defect structure of Ta-substituted Zn2TiO4 oxide ion conductors
Takai, S.; Shinohara, T.; Hoshikawa, A.; Harjo, S.; Oikawa, K.; Ishigaki, T.; Kamiyama, T.; Esaka, T.; Journal of the Ceramic Society of Japan 115 (2007) 780–785; doi:

data_1544562
_publ_section_title
;
 Neutron diffraction study on the defect structure of Ta-substituted
 Zn2TiO4 oxide ion conductors
;
_journal_name_full               'Journal of the Ceramic Society of Japan'
_journal_page_first              780
_journal_page_last               785
_journal_volume                  115
_journal_year                    2007
_chemical_formula_sum            'O4 Ti Zn2'
_chemical_name_common            'Zn2TiO4 cubic spinel'
_space_group_IT_number           227
_space_group_name_H-M_alt        'F d -3 m'
_symmetry_space_group_name_Hall  'F 4d 2 3 -1d'
_symmetry_space_group_name_H-M   'F d -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.46952(8)
_cell_length_b                   8.46952(8)
_cell_length_c                   8.46952(8)
_cell_volume                     607.542(10)
_cod_data_source_file            Zn2TiO4-cubic.cif
_cod_data_source_block           Zn2TiO4-cubic
_cod_original_formula_sum        'Zn2 Ti O4'
_cod_database_code               1544562
Neutron diffraction study on the defect structure of Ta-substituted Zn2TiO4 oxide ion conductors
Takai, S.; Shinohara, T.; Hoshikawa, A.; Harjo, S.; Oikawa, K.; Ishigaki, T.; Kamiyama, T.; Esaka, T.; Journal of the Ceramic Society of Japan 115 (2007) 780–785; doi:

data_1544563
_publ_section_title
;
 Neutron diffraction study on the defect structure of Ta-substituted
 Zn2TiO4 oxide ion conductors
;
_journal_name_full               'Journal of the Ceramic Society of Japan'
_journal_page_first              780
_journal_page_last               785
_journal_volume                  115
_journal_year                    2007
_chemical_formula_sum            'O4 Ta0.12 Ti0.88 Zn1.94'
_chemical_name_common            Zn1.94Ti0.88Ta0.12O4
_space_group_IT_number           227
_space_group_name_H-M_alt        'F d -3 m'
_symmetry_space_group_name_Hall  'F 4d 2 3 -1d'
_symmetry_space_group_name_H-M   'F d -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.48360(6)
_cell_length_b                   8.48360(6)
_cell_length_c                   8.48360(6)
_cell_volume                     610.577(7)
_cod_data_source_file            Zn1.94Ti0.88Ta0.12O4-cubic.cif
_cod_data_source_block           Zn1.94Ti0.88Ta0.12O4-cubic
_cod_original_formula_sum        'Zn1.94 Ti0.88 Ta0.12 O4'
_cod_database_code               1544563
Neutron diffraction study on the defect structure of Ta-substituted Zn2TiO4 oxide ion conductors
Takai, S.; Shinohara, T.; Hoshikawa, A.; Harjo, S.; Oikawa, K.; Ishigaki, T.; Kamiyama, T.; Esaka, T.; Journal of the Ceramic Society of Japan 115 (2007) 780–785; doi:

data_1544564
_publ_section_title
;
 Neutron diffraction study on the defect structure of Ta-substituted
 Zn2TiO4 oxide ion conductors
;
_journal_name_full               'Journal of the Ceramic Society of Japan'
_journal_page_first              780
_journal_page_last               785
_journal_volume                  115
_journal_year                    2007
_chemical_formula_sum            'O4 Ta0.16 Ti0.84 Zn1.92'
_chemical_name_common            'Zn1.92Ti0.84Ta0.16O4 cubic spinel'
_space_group_IT_number           227
_space_group_name_H-M_alt        'F d -3 m'
_symmetry_space_group_name_Hall  'F 4d 2 3 -1d'
_symmetry_space_group_name_H-M   'F d -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.48834(8)
_cell_length_b                   8.48834(8)
_cell_length_c                   8.48834(8)
_cell_volume                     611.601(10)
_cod_data_source_file            Zn1.92Ti0.84Ta0.16O4-cubic.cif
_cod_data_source_block           Zn1.92Ti0.84Ta0.16O4-cubic
_cod_original_formula_sum        'Zn1.92 Ti0.84 Ta0.16 O4'
_cod_database_code               1544564
Neutron diffraction study on the defect structure of Ta-substituted Zn2TiO4 oxide ion conductors
Takai, S.; Shinohara, T.; Hoshikawa, A.; Harjo, S.; Oikawa, K.; Ishigaki, T.; Kamiyama, T.; Esaka, T.; Journal of the Ceramic Society of Japan 115 (2007) 780–785; doi:

data_1544565
_publ_section_title
;
 Neutron diffraction study on the defect structure of Ta-substituted
 Zn2TiO4 oxide ion conductors
;
_journal_name_full               'Journal of the Ceramic Society of Japan'
_journal_page_first              780
_journal_page_last               785
_journal_volume                  115
_journal_year                    2007
_chemical_formula_sum            'O4 Ta0.15 Ti0.85 Zn1.925'
_chemical_name_common            'Zn1.925Ti0.85Ta0.15O4 cubic spinel'
_space_group_IT_number           227
_space_group_name_H-M_alt        'F d -3 m'
_symmetry_space_group_name_Hall  'F 4d 2 3 -1d'
_symmetry_space_group_name_H-M   'F d -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.48707(10)
_cell_length_b                   8.48707(10)
_cell_length_c                   8.48707(10)
_cell_volume                     611.327(12)
_cod_data_source_file            Zn1.925Ti0.85Ta0.15O4-cubic.cif
_cod_data_source_block           Zn1.925Ti0.85Ta0.15O4-cubic
_cod_original_formula_sum        'Zn1.925 Ti0.85 Ta0.15 O4'
_cod_database_code               1544565
Neutron diffraction study on the defect structure of Ta-substituted Zn2TiO4 oxide ion conductors
Takai, S.; Shinohara, T.; Hoshikawa, A.; Harjo, S.; Oikawa, K.; Ishigaki, T.; Kamiyama, T.; Esaka, T.; Journal of the Ceramic Society of Japan 115 (2007) 780–785; doi:

data_1544566
_publ_section_title
;
 Neutron diffraction study on the defect structure of Ta-substituted
 Zn2TiO4 oxide ion conductors
;
_journal_name_full               'Journal of the Ceramic Society of Japan'
_journal_page_first              780
_journal_page_last               785
_journal_volume                  115
_journal_year                    2007
_chemical_formula_sum            'O4 Ta0.14 Ti0.86 Zn1.93'
_chemical_name_common            'Zn1.93Ti0.86Ta0.14O4 cubic spinel'
_space_group_IT_number           227
_space_group_name_H-M_alt        'F d -3 m'
_symmetry_space_group_name_Hall  'F 4d 2 3 -1d'
_symmetry_space_group_name_H-M   'F d -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.48584(7)
_cell_length_b                   8.48584(7)
_cell_length_c                   8.48584(7)
_cell_volume                     611.061(9)
_cod_data_source_file            Zn1.93Ti0.86Ta0.14O4-cubic.cif
_cod_data_source_block           Zn1.93Ti0.86Ta0.14O4-cubic
_cod_original_formula_sum        'Zn1.93 Ti0.86 Ta0.14 O4'
_cod_database_code               1544566
Neutron diffraction study on the defect structure of Ta-substituted Zn2TiO4 oxide ion conductors
Takai, S.; Shinohara, T.; Hoshikawa, A.; Harjo, S.; Oikawa, K.; Ishigaki, T.; Kamiyama, T.; Esaka, T.; Journal of the Ceramic Society of Japan 115 (2007) 780–785; doi:

data_1544567
_publ_section_title
;
 Neutron diffraction study on the defect structure of Ta-substituted
 Zn2TiO4 oxide ion conductors
;
_journal_name_full               'Journal of the Ceramic Society of Japan'
_journal_page_first              780
_journal_page_last               785
_journal_volume                  115
_journal_year                    2007
_chemical_formula_sum            'O4 Ta0.1 Ti0.9 Zn1.95'
_chemical_name_common            'Zn1.95Ti0.9Ta0.1O4 cubic spinel'
_space_group_IT_number           227
_space_group_name_H-M_alt        'F d -3 m'
_symmetry_space_group_name_Hall  'F 4d 2 3 -1d'
_symmetry_space_group_name_H-M   'F d -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.48705(12)
_cell_length_b                   8.48705(12)
_cell_length_c                   8.48705(12)
_cell_volume                     611.322(15)
_cod_data_source_file            Zn1.95Ti0.9Ta0.1O4-cubic.cif
_cod_data_source_block           Zn1.95Ti0.9Ta0.1O4-cubic
_cod_original_formula_sum        'Zn1.95 Ti0.9 Ta0.1 O4'
_cod_database_code               1544567